# Ab Initio and Experimental Techniques for Studying Non Stoichiometry and Oxygen Transport in Mixed Conducting Oxides

0

1

143

1 month ago

PDF Preview

Full text

(2) ii. © 2014 Chirranjeevi Balaji Gopal All Rights Reserved.

(3) iii. Acknowledgments My life as a graduate student at Caltech has been nothing short of life-changing and I owe this to a lot of people. First out, my parents have always put my ambitions and interests above all else and backed me to come to Caltech. I am tremendously grateful to my advisers, Axel van de Walle and Sossina Haile for mentoring me through the years. Transitioning from simulations to full-blown experiments requires patience, trust and genuine excitement from the adviser. Sossina supported me with all this and much more. I met some really smart, inspiring and yet humble people here, many of who have had a lasting influence on my life. In particular, I can’t thank Cindy enough for the personal and academic support she provided me with and numerous life lessons in my formative years here. Aron and Steve, with their towering brilliance and (periodically) near-juvenile maturity, made my time at Caltech intellectually stimulating and fun in equal measure. I am also grateful to PT, Alex(s), Himanshu, Christina, Joel, Vanessa and many more friends for making me feel home at work. These are all wonderful people that I would like to always be in touch with. Thanks to the caltech alpine club, I got hooked to mountains, snow, and other outdoorsy pursuits that are borderline suffer-fests on occasions and met many a colorful character. I would also like to acknowledge my colleagues from Axel’s group - PT, Steve, Qijun, Greg and Ljuba for many engaging discussions - scientific or otherwise. These are among the smartest people I have come to know. Big thanks to Aron, William, Tae-sik, Yong, Woochul and other Haile group members for helping me get set in the lab. I would also like to thank Arun, my SURF student for some great work in the summer of 2012. Thanks to Anu and Vanessa for proofreading parts of the thesis..

(4) iv Caltech is truly a remarkable place to mature as a scientist and I feel very fortunate to have been in such good academic company. Lastly, but very importantly, I would like to express my love and gratitude to Jenny for the unconditional love, joy and encouragement she has offered me over the last year and making me realize what is truly valuable in life..

(5) v Portions of this thesis have been adapted with permission from the following sources in which I am the first author. • Chirranjeevi Balaji Gopal and Axel van de Walle, Ab initio thermodynamics of intrinsic oxygen vacancies in ceria, Physical Review B, 86, 13, 134117, 2012 • Chirranjeevi Balaji Gopal and Sossina M Haile, An electrical conductivity relaxation study of oxygen transport in samarium doped ceria, Journal of Materials Chemistry A, 2, 7, 2405-2417, 2014 • Chirranjeevi Balaji Gopal, Arun Asundi and Sossina M Haile, Effect of Zr addition on oxygen transport in ceria : an electrical conductivity relaxation study, (in preparation) • Chirranjeevi Balaji Gopal and Sossina M Haile, Electrochemical determination of non-stoichiometry in mixed conducting oxide thin films, (in preparation) • Chirranjeevi Balaji Gopal and Sossina M Haile, Membrane reactor for thermochemically driven fuel production, Provisional Patent, CIT-6744-P.

(6) vi. Abstract The ability of cerium oxide (CeO2−δ , also called ceria), to vary its oxygen stoichiometry in response to changes in temperature or oxygen activity is key to many of its applications in catalysis and electrochemical energy storage and conversion. This thesis explores ab initio and experimental approaches to study the fundamental thermodynamic and oxygen transport properties of ceria (Mx Ce1−x O2−δ ), but the methods are applicable to other mixed conducting oxides as well. In the first part of the thesis, a computational thermodynamics approach that integrates quantum mechanical and statistical ensemble-based simulations is used to calculate the reduction-oxidation thermodynamics of non-stoichiometric ceria entirely from first principles. This procedure is well understood and has been successfully implemented for metallic alloys, but has not been extended to correlated electron systems such as ceria, for which the physics of electronic structure calculations is significantly more complicated. Density functional calculations were used to obtain the ground state energies of ceria with vacancy concentrations ranging from fully stoichiometric up to δ = 0.25. For each δ, numerous vacancy configurations were sampled to capture the interactions between vacancies and other atoms. Using the frozen phonon method, lattice dynamical calculations of phonon density of states were performed for various δ. Based on the ground state energies of nearly 40 structures, a cluster expansion Hamiltonian was used to parametrize the energy as a polynomial in occupation variables. The vibrational energies were used to make the Hamiltoninan temperature dependent. Lattice Monte Carlo (MC) simulations using the cluster expansion Hamiltonian were then used to study, for the first time, the effect of temperature and chemical potential on the vacancy concentration in ceria from first principles..

(7) vii The temperature composition phase diagram constructed from the MC simulations successfully reproduced the experimentally reported miscibility gap. The inclusion of vibrational and electronic contributions to the entropy made the agreement quantitative. Further, the partial molar enthalpy and entropy of reduction as a function of δ were extracted and found to deviate significantly from those of an ideally behaved system. The deviations were quantified by calculating the Warren-Cowley short range order parameters. This was the first demonstration of an ab initio approach being used to accurately model the defect thermodynamics of a correlated electron system without resorting to experimental inputs. Using ceria as benchmark material, this project lays the groundwork for a computational approach to screen new oxides for thermochemical cycling. The rest of the thesis describes experimental investigations of oxygen transport and non-stoichiometry in doped and undoped ceria. Oxygen transport studies were performed using electrical conductivity relaxation (ECR). In ECR, a small step change in pO2 forces the sample non-stoichiometry δ, and other dependent properties such as electrical conductivity, to equilibrate to a new value. The rate of this re-equilibration is governed by the bulk oxygen diffusivity, DChem , and surface reaction rate constant, kS – the two principal kinetic properties. By fitting the solution to Fick’s second law, with the appropriate boundary conditions, to the conductivity relaxation profile, DChem and kS can be extracted. The instrumental capability for performing electrical conductivity relaxation experiments was set up and a systematic data analysis procedure was developed to reliably and accurately extract DChem and or kS . The experimental and data analytical methodologies were successfully benchmarked with 15 mol% Sm doped ceria, for which approximate values of the two principal transport properties, bulk oxygen diffusivity, DChem , and surface reaction rate constant, kS , can be found in the literature. An unexpectedly high p-type electronic transference number enabled ECR measurements under oxidizing conditions. A systematic data analysis procedure was developed to permit reliable extraction of the kinetic parameters even in the general case of simultaneous bulk and surface limitation. When the surface kinetics were too sluggish compared to bulk diffusion, Pt catalyst nanoparti-.

(8) viii cles were sputtered to catalyze the surface reaction and enable extraction of DChem . The DChem from this study showed excellent qualitative and quantitative agreement with expected values, falling in the range from ∼ 2 × 10−5 to 2 × 10−4 cm2 /s. The surface reaction constant under H2 /H2 O mixtures also showed good agreement with literature results. Remarkably, this value increased by a factor of 40 under mixtures of CO/CO2 or O2 /Ar. This observation suggests kinetic advantages for production of CO rather than H2 in a two-step solar-driven thermochemical process based on samarium doped ceria. Using ECR, the effect of 20% Zr addition on the electrical conductivity and oxygen transport properties of ceria as a function of pO2 and T was investigated. Under oxidizing conditions, both CeO2−δ and Zr0.2 Ce0.8 O2−δ (ZDC20) showed n type, mixed conduction. The conductivity of ZDC20 was two orders of magnitude higher than that of undoped ceria. Contrary to previous studies, we found that Zr addition does not change the electronic mobility in this pO2 regime. The enhancement in conductivity is a consequence of higher vacancy concentration in ZDC20 under identical conditions compared to ceria. Under reducing conditions, while the n-type conductivity of ceria continued to increase with decreasing pO2 , that of ZDC20 reached a broad maximum, eventually decreasing with pO2 (p-type) despite increasing carrier concentration. We show that the electronic mobility becomes strongly concentration dependent at high oxygen non-stoichiometry. This leads to a marked decrease in mobility with increase in δ, causing the conductivity to roll over from n to p type. The chemical diffusion coefficient and surface reaction rate constant of both ceria and ZDC20 showed strong dependence on pO2 under oxidizing conditions, decreasing by nearly an order of magnitude between 10−2 atm and 10−5 atm. The unexpectedly high sensitivity to pO2 was ascribed to the effect of extrinsic vacancies generated by trace quantities of lower valence cation impurities, that dramatically increase both the absolute value of the thermodynamic factor and its sensitivity to pO2 close to stoichiometry. Overall, the addition of Zr lowers the DChem and kS of ceria in the temperature and oxygen partial pressure range of this study, the effect being more pronounced under reducing conditions. Beyond its relevance to ceria, this work demonstrates the potential of.

(9) ix ECR to isolate the effect of kinetics from thermodynamics of the real thermochemical cycle, reveal the limiting transport parameters, and ultimately guide microstructure design for maximizing the rate of fuel production. Lastly, we improve upon an existing formalism to calculate the oxygen nonstoichiometry in thin films of mixed conducting oxides using AC impedance spectroscopy. Cerium oxide was once again chosen as the benchmarking material, since it shows both ideal and non-ideal thermodynamic behavior under different conditions, and has been well studied in its bulk form. In this method, the impedance response of dense, thin films of CeO2−δ deposited on a Y0.84 Zr0.16 O1.92 (YSZ) substrate was measured using AC impedance spectroscopy. To explore potential grain boundary effects on bulk thermodynamic properties. A physically derived equivalent circuit model was fit to the impedance response to extract a quantity called the ‘chemical capacitance’, which was subsequently related to the non-stoichiometry. Previous studies employing this method were restricted to systems that can be described using ideal solution thermodynamics, which allows simplifications to the theoretical treatment of their capacitance. Apart from extending this technique to a non-ideally behaved oxide, we report excellent agreement between the non-stoichiometry of single crystal and polycrystalline films and that of bulk ceria. By virtue of using thin films, equilibration times are dramatically decreased, enabling faster measurements compared to bulk techniques like thermogravimetry and coulometric titration. Further, the electrochemical method is ideal for thin films, for which the mass changes are below the detection limits of bulk techniques..

(10) x. Contents Acknowledgments. iii. Abstract. vi. List of Figures. xiii. List of Tables. xvii. 1 Introduction and background. 1. 1.1. Big picture. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 1. 1.2. Storing solar energy in chemical bonds . . . . . . . . . . . . . . . . .. 2. 1.3. Thermochemical water splitting using CeO2−δ . . . . . . . . . . . . .. 4. 1.4. Motivation and outline . . . . . . . . . . . . . . . . . . . . . . . . . .. 5. 2 Vacancy thermodynamics in ceria using first principles calculations. 8. 2.1. Why computational thermodynamics ? . . . . . . . . . . . . . . . . .. 8. 2.2. Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 10. 2.3. Methodology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 12. 2.3.1. First principles calculations . . . . . . . . . . . . . . . . . . .. 13. 2.3.2. Cluster expansion : configurational degrees of freedom . . . .. 15. 2.3.3. Lattice Monte Carlo simulations : thermodynamic properties .. 16. Results and discussion . . . . . . . . . . . . . . . . . . . . . . . . . .. 18. 2.4.1. First principles calculations . . . . . . . . . . . . . . . . . . .. 18. 2.4.2. Cluster expansion . . . . . . . . . . . . . . . . . . . . . . . . .. 19. 2.4.3. Monte Carlo simulations . . . . . . . . . . . . . . . . . . . . .. 20. 2.4.

(11) xi 2.5. Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 29. 3 An electrical conductivity relaxation study of oxygen transport in samarium doped ceria. 31. 3.1. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 31. 3.2. Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 33. 3.2.1. Electrical conductivity relaxation . . . . . . . . . . . . . . . .. 33. 3.2.2. Defect chemistry and conductivity of SDC15 . . . . . . . . . .. 36. 3.2.3. Chemical diffusion coefficient . . . . . . . . . . . . . . . . . .. 38. 3.2.4. Surface reaction rate constant . . . . . . . . . . . . . . . . . .. 41. Experimental and analytical procedure . . . . . . . . . . . . . . . . .. 43. 3.3.1. Experimental methods . . . . . . . . . . . . . . . . . . . . . .. 43. 3.3.2. Analysis of relaxation data . . . . . . . . . . . . . . . . . . . .. 47. Results and discussion . . . . . . . . . . . . . . . . . . . . . . . . . .. 53. 3.4.1. Equilibrium conductivity . . . . . . . . . . . . . . . . . . . . .. 53. 3.4.2. Relaxation behavior. . . . . . . . . . . . . . . . . . . . . . . .. 55. Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 61. 3.3. 3.4. 3.5. 4 Effect of Zr addition on transport properties of ceria : an electrical conductivity relaxation study. 63. 4.1. Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 63. 4.2. Defect chemistry of undoped ceria . . . . . . . . . . . . . . . . . . . .. 65. 4.3. Experimental procedure . . . . . . . . . . . . . . . . . . . . . . . . .. 69. 4.4. Results and discussion . . . . . . . . . . . . . . . . . . . . . . . . . .. 69. 4.4.1. Equilibrium conductivity . . . . . . . . . . . . . . . . . . . . .. 69. 4.4.2. Oxygen transport . . . . . . . . . . . . . . . . . . . . . . . . .. 74. Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 82. 4.5. 5 Eletrochemical determination of oxygen non-stoichiometry in mixed conducting oxide thin films. 84. 5.1. 84. Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . ..

(12) xii 5.2. 5.3. 5.4. 5.5. Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 86. 5.2.1. Derivation of chemical capacitance . . . . . . . . . . . . . . .. 87. 5.2.2. From chemical capacitance to non-stoichiometry . . . . . . . .. 88. 5.2.3. AC impedance spectroscopy . . . . . . . . . . . . . . . . . . .. 90. Experimental methods . . . . . . . . . . . . . . . . . . . . . . . . . .. 91. 5.3.1. Sample preparation and characterization . . . . . . . . . . . .. 91. 5.3.2. Electrochemical measurements . . . . . . . . . . . . . . . . . .. 95. Results and discussion . . . . . . . . . . . . . . . . . . . . . . . . . .. 95. 5.4.1. Impedance spectra and equivalent circuit modeling . . . . . .. 95. 5.4.2. Chemical capacitance . . . . . . . . . . . . . . . . . . . . . . . 100. 5.4.3. Non-stoichiometry from chemical capacitance . . . . . . . . . 102. Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105. A Fits to partial molar oxygen enthalpy and entropy of ceria. 106. B Electrical conductivity relaxation studies of ceria and ZDC20 under isothermal cycling conditions. 108. B.1 Background . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 108 B.2 Conductivity at 1400 ◦ C . . . . . . . . . . . . . . . . . . . . . . . . . 110 B.3 Relaxation behavior . . . . . . . . . . . . . . . . . . . . . . . . . . . . 110 C Thermodynamic integration to obtain reference state. 114. Bibliography. 118.

(13) xiii. List of Figures 1.1. Unit cell of ceria . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 1.2. Illustration of a two step solar thermochemical cycle to split water and. 4. produce hydrogen. . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 5. 2.1. 2 × 2 × 2 supercell of stoichiometric ceria. . . . . . . . . . . . . . . . .. 13. 2.2. 2 × 2 × 2 supercells of ceria with different vacancy content . . . . . . .. 14. 2.3. Plot of the convex hull of various defect structures . . . . . . . . . . .. 19. 2.4. Calculated phonon density of states for CeO2−δ . . . . . . . . . . . . .. 20. 2.5. Effective cluster interactions vs cluster diameter . . . . . . . . . . . . .. 21. 2.6. Temperature oxygen non-stoichiometry plot for a constant µ Monte Carlo simulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 2.7. 23. Calculated high temperature phase diagram of CeO2−δ with and without vibrational entropy effects. . . . . . . . . . . . . . . . . . . . . . . . . .. 24. 2.8. Entropy of CeO2−δ computed from Monte Carlo simulations . . . . . .. 25. 2.9. Entropy of reduction as a function of δ from Monte Carlo simulations .. 26. 2.10. Possible vacancy pairs . . . . . . . . . . . . . . . . . . . . . . . . . . .. 27. 2.11. Warren Cowley short range order parameters for vacancy pair clusters.. 29. 3.1. Scanning electron micrograph of a sintered SDC15 pellet . . . . . . . .. 43. 3.2. Scanning electron micrograph of Pt catalyst particles sputtered on SDC15 sample . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 3.3 3.4. 43. Illustration of data analytical procedures developed to extract DChem and kS from conductivity relaxation data . . . . . . . . . . . . . . . . .. 44. Evaluation of numerical procedures developed for analyzing ECR data. 47.

(14) xiv 3.5. Residuals from fitting 2D and 1D diffusion model to conductivity relaxation profiles . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 47. 3.6. Log-log plot of electrical conductivity of SDC15 vs pO2 . . . . . . . . .. 50. 3.7. Raw and normalized conductivity relaxation profiles along reducing and oxidizing directions for SDC15 . . . . . . . . . . . . . . . . . . . . . . .. 3.8. Comparison of conductivity relaxation profiles with and without Pt catalyst decoration on the surface of an SDC15 sample . . . . . . . . . . .. 3.9. 55. Raw conductivity and pO2 vs time for an SDC15 sample under oxidizing conditions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 3.11. 53. Effect of gas phase composition on the conductivity relaxation profile of SDC15 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 3.10. 51. 56. DChem of SDC15 from conductivity relaxation experiments compared with theoretical estimates based on an ideal solution model. . . . . . .. 58. 3.12. DChem of SDC15 from conductivity relaxation experiments. . . . . . .. 59. 4.1. Log-log plot of electrical conductivity vs pO2 for ceria and ZDC20 . . .. 71. 4.2. Partial ionic and electronic conductivity of ceria and ZDC20 under oxidizing conditions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 71. 4.3. Electrical conductivity of ceria and ZDC20 vs non-stoichiometry at 800◦ C. 73. 4.4. Comparison of ECR profiles along oxidizing and reducing directions to determine the validity of small pO2 step change . . . . . . . . . . . . .. 74. 4.5. Raw ECR profiles at 2.8 × 10−1 atm and 8 × 10−4 atm pO2. 75. 4.6. DChem vs pO2 at 750◦ C, 800◦ C and 850◦ C for undoped ceria and ZDC20 75. 4.7. kS vs pO2 at 750◦ C, 800◦ C and 850◦ C for undoped ceria and ZDC20 .. 76. 4.8. Fit to experimentally measured ∆HO and ∆SO . . . . . . . . . . . . .. 77. 4.9. Re-calculated δ-pO2 isotherms at 800◦ C for undoped ceria in the presence of varying impurity levels. 4.10. . . . . . .. . . . . . . . . . . . . . . . . . . . . . .. 78. Effect of lower valence impurities on the thermodynamic factor of undoped ceria . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 79.

(15) xv 5.1. A simulated Nyquist plot for charge transport involving conduction through the grains and grain boundaries and an electrochemical reaction at the electrode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 5.2. 2θ − ω coupled scan of a 500 nm film of ceria deposited on a (001) oriented YSZ substrate. . . . . . . . . . . . . . . . . . . . . . . . . . .. 5.3. 93. Pole figure measurements of 200 and 220 reflections of a ceria thin film deposited on single crystal YSZ . . . . . . . . . . . . . . . . . . . . . .. 5.4. 92. 93. SEM images of ceria films deposited on single crystal and polycrystalline YSZ substrates. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 94. 5.5. SEM image of porous, inter-connected Pt current collector . . . . . . .. 94. 5.6. Typical impedance spectra under reducing conditions . . . . . . . . . .. 96. 5.7. Offset resistance as a function of oxygen partial pressure and temperature. 97. 5.8. Arrhenius plot of the electrical conductivity of the YSZ susbtrate . . .. 5.9. Temperature and oxygen partial pressure dependence of the electro-. 97. chemical reaction resistance . . . . . . . . . . . . . . . . . . . . . . . .. 98. 5.10. Typical impedance spectra under oxidizing conditions. . . . . . . . . .. 99. 5.11. Separating interfacial and bulk capacitance. . . . . . . . . . . . . . . . 100. 5.12. Chemical capacitance vs oxygen partial pressure extracted from the impedance response . . . . . . . . . . . . . . . . . . . . . . . . . . . . 101. 5.13. Non-stoichiometry as a function of oxygen partial pressure under reducing conditions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 103. B.1. Log-log plot of conductivity of ceria and ZDC20 vs pO2 at 1400◦ C . . . 109. B.2. Sample ECR profile at 1400 ◦ C and a step change from pO2 = 10−3 atm to 5 × 10−4 atm for a 0.5 mm thick ceria sample . . . . . . . . . . . . . 111. B.3. ECR profile for a pO2 step change from 10−4 to 1.4 × 10−4 atm using wet and dry atmospheres. . . . . . . . . . . . . . . . . . . . . . . . . . 112. B.4. kS vs pO2 for undoped ceria and ZDC20 at 1400◦ C . . . . . . . . . . . 113. B.5. ECR profiles of undoped ceria for large step changes.. C.1. Iso-δ plots of µO vs T to illustrate the reference state calculation procedure.115. . . . . . . . . . 113.

(16) xvi C.2. Slopes of linear fits to iso-δ plots of µO vs T overlaid on a plot of ∆Sconf ig vs δ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 115.

(17) xvii. List of Tables 2.1. Types and coordinates of clusters identified by the cluster expansion fit.. 3.1. Representative results from testing the data analysis routine on datasets. 28. generated with known values of sample thickness (2a = 0.1 cm), chemical diffusion coefficient (DChem cm2 /s) and surface reaction rate constant (kS cm/s). Superscript ‘only’ indicates fits performed using the relevant one-parameter model. . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2. 45. Parameters describing the conductivity of SDC15, based on a fit of the expression in Equation 3.31 to determine the ionic, n-type, and p-type conductivities, as well as fit to an Arrhenius expression (σT = A exp(−Ea /kb T )). . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 54. 4.1. Electronic mobility of ceria and ZDC20 . . . . . . . . . . . . . . . . . .. 72. A.1. The partial molar entropy of reduction of ceria (units of J/K/mol of oxygen vacancies) obtained from the work of Panlener et al.[1]. . . . . 106. A.2. The partial molar enthalpy of reduction of ceria (units of kJ/mol of oxygen vacancies) obtained from the work of Blumenthal et al.[2]. It was fit using a cubic hermite interpolating polynomial. . . . . . . . . . 107.

(18) 1. Chapter 1 Introduction and background 1.1. Big picture. Fossil fuels, comprising coal, natural gas and petroleum, are the primary source of energy in the modern world. The high energy density of these carbon rich compounds and the ability to easily store and transport them, has spearheaded the industrial and economic development of entire societies worldwide. As of 2012, 82%[3] of the total energy use in the United States was supplied by fossil fuels. However, fossil fuels take millions of years to form, and known, viable reserves are being depleted much faster than new ones are being created. Moreover, indiscriminate use of fossil fuels has drastically increased the concentration of greenhouse gases in the atmosphere, contributing to global climate disruption and worsening air quality. At 26%, the burning of coal, natural gas, and oil for electricity is the single largest source of greenhouse gas emissions globally[3]. This has led to the need for sustainable energy solutions to help ease the dependence on, if not facilitate a complete removal from fossil energy. Solar energy is virtually inexhaustible and is the biggest renewable energy source available to us. At any instant, 176000 terawatts of solar radiation strikes the earth. In comparison, the global power consumption, as of 2012, was 16 terawatts. If only 0.1% of the incident solar energy were to be utilized at 10% efficiency, we would meet the global energy needs using solar[4]. However, proliferation of solar power generation has been limited by lack of effective storage technologies. Thus, one of.

(19) 2 the biggest objectives of sustainable energy research is developing a means to harvest and store solar energy and make it available for use when necessary.. 1.2. Storing solar energy in chemical bonds. Storing energy in chemical bonds is highly attractive for the same reasons that fossil fuels are extremely sought after – high energy density, ease of storage and transportation, and demand based use. Efforts are being made world wide to improve the energy density of batteries for efficient storage of electricity and to develop efficient and economically viable methods of hydrogen production from water. Hydrogen is an excellent and clean fuel, whose utilization produces water as the only waste product. There are a variety of ways to produce hydrogen, each with its own merits and demerits. Thermolysis using concentrated solar radiation is the most direct means of dissociating steam and generating hydrogen. However, to dissociate 50% of the water molecules, temperatures in excess of 3000 ◦ C are necessary, placing severe requirements on the materials used to engineer such a device. Another possible route is to convert solar energy to electricity using photovoltaic cells, which could then be used to power an electrolyzer for water electrolysis. Rapid strides are being made to improve the efficiency of photovoltaics and to develop better water oxidation catalysts. By combining the light harvesting and water splitting steps using a photoelectrochemical cell, significant reduction in capital costs and improvement in system efficiency can be achieved. Despite the advantage of low temperature operation, photoelectrochemical cells use only a limited portion (visible, UV) of the solar spectrum, require exotic catalysts and suffer from serious material limitations. In this regard, photoactive semiconductors with desirable band gap, band alignment with the electrochemical potentials for oxygen/hydrogen evolution reactions, rapid charge transfer kinetics and long term stability in aqueous media are being actively researched. There are several excellent reviews describing the concepts and recent developments in the field, dubbed ‘artificial photosynthesis’[5] and identifying the design constraints and research breakthroughs that are necessary to make solar water-splitting cells com-.

(20) 3 mercially viable[6]. An alternate approach is to use solar energy to thermochemically split water using the redox active nature of certain metal oxides. The process is typically carried out in two steps. First, concentrated solar energy is used to release oxygen from the metal oxide by partially or completely reducing it at a high temperature step. In the second step, the reduced metal oxide or metal is re-oxidized back to the original state by reacting it with steam (H2 O), generating hydrogen (H2 ). Hydrogen, together with carbon dioxide, can subsequently be used as a feedstock for the Fischer Tropsch process to produce methane, or can be delivered to fuel cells to produce electricity. Metal-metal oxide based redox systems (e.g. Zn/ZnO, FeO/Fe3 O4 ) have been been studied for over 35 years[7, 8, 9, 10]. The large gravimetric changes associated with complete reduction of the oxide translate to large theoretical fuel productivities. However, there are considerable engineering challenges and kinetic impediments due to extremely high reduction temperatures (>2500 K), the formation of an impervious oxide layer on the surface, and the need to use nanoparticles for reaction sufficient kinetics[11]. To prevent aggressive coarsening of particles at elevated temperatures, catalyst supports such as zirconia are used at the cost of lower gravimetric fuel producivity[12] (since zirconia is redox-inactive). Most of these shortcomings are overcome using thermochemical cycles based on non-stoichiometric oxides. In non-stoichiometric oxides, only a fraction of the stoichiometric quantity of oxygen is released and reincorporated, implying lower fuel productivity per cycle compared to completely reduced oxides, but the oxygen exchange occurs without loss of the original crystal structure. Further, a number of non-stoichiometric oxides are well known for their high temperature stability, excellent surface activity for oxygen exchange and bulk oxygen diffusivity in other applications such as solid oxide fuel cells, oxygen sensors and oxygen storage catalysts[13, 14, 15]. The combination of all these properties make a strong case for thermochemical water splitting based on the redox behavior of non-stoichiometric oxides. In particular, cerium oxide (CeO2 ) is an excellent candidate, since it satisifies the aforementioned criteria[16, 17] and cerium (despite being classified a rare-earth element) is as earth abundant as copper - an.

(21) 4 important economic advantage for scalability.. 1.3. Thermochemical water splitting using CeO2−δ. Ceria, CeO2 , crystallizes in the cubic fluorite structure (Fig. 1.1), with the oxygen ions (O2− ) occupying the tetrahedral voids in the face centered cubic lattice of cerium ions (Ce4+ ). Under reducing conditions, achieved either by heating the oxide and/or reducing the oxygen activity in the environment, a fraction of the oxygen atoms is released from the structure to equilibrate the chemical potential of oxygen in the gas and solid phase. This re-equilibration leads to creation of bulk oxygen vacancies, charge compensated by the conversion of twice as many Ce4+ to Ce3+ . In fact, at temperatures above 1000 ◦ C, up to δ ≈ 0.25 can be generated within the cubic fluorite structure of CeO2−δ [18]. In a two step thermochemical cycle, schematically depicted. Ce. O. Figure 1.1: Cubic fluorite unit cell of stoichiometric ceria, CeO2 . The oxygen ions sit in the tetrahedral voids of a face centered cubic lattice of cerium ions. in Fig. 1.2, ceria is first thermally reduced at 1500 ◦ C or above in an inert atmosphere, followed by hydrolysis at 800 ◦ C to liberate hydrogen, T. H CeO2−δL −→ CeO2−δH +. δH − δL O2 , 2 T. L CeO2−δH + (δH − δL )H2 O −→ CeO2−δL + (δH − δL )H2 .. (1.1) (1.2).

(22) 5 δL and δH respectively denote the oxygen non-stoichiometry at the low temperture. Reduction TH. Hydrolysis TL CO2 H2 O. H2 O. 2 2. CeO2. CeO2. H. 2. O2. L. CO. Figure 1.2: Illustration of a two step solar thermochemical cycle that uses nonstoichiometric ceria to split water and produce hydrogen. δL and δH respectively denote the oxygen non-stoichiometry at the low temperature (TL ) and high temperature (TH ) steps, and ∆δ = δH − δL (TL ) and high temperature (TH ) steps, and δL is typically ∼ 0. A similar reaction scheme can be constructed for dissociation of carbon dioxide (CO2 ), which generates carbon monoxide (CO) at temperatures high enough to inhibit carbon formation. The process variables - temperature and oxygen partial pressure in the carrier gas - are chosen to maximize the fuel productivity and production rates. The feasibility of a ceria-based thermochemical process to split water has been demonstrated successfully[19, 20, 21, 22]. Fuel productivities of up to 11.8 ml hydrogen per gram of ceria at 6.2 ml per gram per minute have been achieved and a closed system efficiency analysis reveals that solar-to-fuel conversion efficiencies of up to 19% can be obtained even without solid state heat recovery[21].. 1.4. Motivation and outline. Maximizing the solar-to-fuel conversion efficiency of a thermochemical cycle requires a multidisciplinary approach. From an engineering perspective, important considerations include efficient solar concentrators that can achieve the desired heat flux, reactor components capable of handling repeated thermal cycling and high temper-.

(23) 6 atures, and minimization of heat losses. The “material specific properties” can be broadly classified into thermodynamic and kinetic. The fuel productivity per cycle is the important thermodynamic criterion, and is governed by the change in equilibrium non-stoichiometry between the reduction and hydrolysis steps, i.e. ∆δ = δH − δL . The non-stoichiometry, δ, is a function of the oxygen partial pressure, pO2 , and temperature, T , and is related to the enthalpy and entropy of reduction. It contains all relevant information about the redox thermodynamics of the system and provides the basis for predicting the equilibrium gravimetric fuel productivity under a given choice of cycling conditions. The goal is to maximize the thermodynamic driving force (increase ∆δ) without compromising the rate of fuel production – the other important metric. Both the oxygen release and water dissociation steps require serial steps of (i) oxygen diffusion through the bulk of the solid, and (ii) surface reaction involving transport of oxygen across the gas-solid interface. The bulk diffusion of oxygen is quantified by the chemical diffusion coefficient, DChem , and the surface transport is quantified by the surface reaction rate constant, kS . Unlike DChem , which is a material property and hence a function of the oxygen activity and temperature only, kS also depends on the gas phase composition (not just pO2 ), surface morphology and surface composition. In principle, the fuel production curves from a thermochemical cycling experiment embody all the material specific parameters. However, the large driving forces (i.e. large changes in T and pO2 ), porous microstructures and poorly controlled gas flow dynamics convolve thermodynamic and kinetic effects, precluding a meaningful comparison of the kinetic properties of candidate materials. Experiments aimed at directly and quantitatively revealing the kinetic properties must use small perturbations from equilibrium to avoid non-linear effects, employ well-defined sample geometries, and present well-controlled gas flow dynamics. A physical understanding of the redox thermodynamics and oxygen transport is essential to rationally guide the search for newer and better performing materials. This work explores state-of-the-art simulations - bridging the gap between quantum mechanical and statistical mechanical calculations - and electrochemical measurements to determine oxygen non-stoichiometry in undoped ceria. It also improves upon.

(24) 7 an established experimental technique for measuring transport properties, to enable a systematic study of the effect of dopants on the behavior of ceria. In Chap. 2, ab initio calculations are integrated with lattice Monte Carlo simulations to predict, for the first time, the phase diagram and macroscopic thermodynamic properties such as reduction enthalpy and entropy of ceria as a function of non-stoichiometry and temperature and short range order parameters, entirely from first principles. In Chap. 3, the versatility of the electrical conductivity relaxation (ECR) technique to quantitatively extract the transport properties of an oxide is demonstrated, using 15 mol% Sm doped ceria as the reference material. A systematic data-analysis procedure was developed to reliably and uniquely determine the chemical diffusivity and/or surface reaction rate constants without making prior assumptions about the nature of the transport process (surface vs bulk vs co-limited). The experimental and data analytical methodologies were then used to study the effect of Zr doping on the eletrical conductivity and oxygen transport properties of ceria, the results of which are discussed in Chap. 4. In Chap. 5, the focus reverts back to thermodynamics. We demonstrate the capability to calculate the bulk non-stoichiometry of oxide thin films using electrochemical measurements. Cerium oxide was once again used as the benchmark material, since it displays both ideal and non-ideal thermodynamic behavior under different environmental conditions and is a well studied system in the literature. Aside from providing greater precision and resolution relative to conventional gravimetric methods of determing defect densities, electrochemical studies on well-defined sample geometries can yield interfacial thermodynamic properties as well. The appendix includes some recent results from ECR studies of ceria and Zr doped ceria at 1400 ◦ C under both small driving forces and large driving forces representative of thermochemical cycling conditions. Each chapter is self contained, in that, the necessary background, theory and experimental details are first presented before discussing the results..

(25) 8. Chapter 2 Vacancy thermodynamics in ceria using first principles calculations 2.1. Why computational thermodynamics ?. Experimentation based science has been the norm for centuries. Existing tools have been constantly refined and newer, sophisticated ones have been developed to push the boundaries of what is measurable. Characterization of sub angstrom length scales and femtosecond timescales are within the realm of experiments today. On the other hand, computers are a relatively new addition to our repertoire of scientific tools. A key advantage of computer simulations is the absolute and precise control that the user possesses over the system variables. Everything starts out ideal unless made otherwise. Testing conditions which are impractical or hazardous to attempt in a lab can be safely obtained in a simulation. Borrowing Prof Cosma Shalizi’s quote, “no one gets wet in a simulated thunderstorm”. Also unique to simulations is the ability to isolate and selectively probe one of many mechanisms that could explain an experimental observation. For instance, the use of zinc phosphide as a low cost, high efficiency photovoltaic material has been limited by the difficulty in n-type doping it. While the synthesis and processing conditions can be varied in anticipation of a desired physical property, computer simulations are necessary to explain the atomistic mechanism linking the electronic structure and processing to the observed experimental result. In case of zinc phosphide, based on the formation energies of all.

(26) 9 possible point defects computed using density functional theory, it was revealed that phosphorus interstitials are thermodynamically favored in the n-type regime, which act as electron sinks and nullify the intended doping effect[23]. Despite their many advantages, computational methods have largely served to validate or support experimental observations in place of predicting new properties or discovering new materials. This is because simulations rely on a physical model and to date, there is not a single model spanning all the length scales and time scales of known physical processes. One option is to resort to quantum mechanics and solve for the wave function of a system, using what are called first principles calculations. The all-electron wave function provides a complete description of the system and can be used to extract the thermodynamic properties across all length scales. Unfortunately, the computational cost of first principles calculations scale rapidly with the number of electrons in the system, and become prohibitively large beyond a few tens of unit cells even for modern supercomputers. Hence, any calculation aimed at investigating macroscopic properties of a system needs some abstractions to transition across the length scales while preserving the underlying physics of problem. For non-stoichiometric ceria, the workhorse of this thesis, the thermodynamics of vacancies are of practical interest only at temperatures over 600 ◦ C and low oxygen activities. As such, the DFT formalism is implemented at absolute zero, so any attempt to model entropic contributions (which favor defects) would need an abstraction to incorporate finite temperature effects. Further, experimentally measurable equilibrium properties such as entropy and enthalpy of reduction and non-stoichiometry at a given pO2 are ensemble averages over a large number of configurations. Thus, a second level of abstraction is needed to include the configurational degrees of freedom. These abstractions have been proposed and initially implemented for metallic alloys, which are substantially simpler systems to model physically. Extending these methods to ceria and other such non-stoichiometric oxides pushes the boundaries of the computational thermodynamics approach and is the focus of this chapter..

(27) 10. 2.2. Background. Significant research has been devoted to understanding the electronic structure of nonstoichiometric ceria from first principles using density functional theory (DFT)[24, 25] with the standard local density approximation (LDA) and generalized gradient approximation (GGA) exchange correlation functionals. It is well known that the 4f electrons in CeO2 need to be treated as valence states to accurately reproduce the experimentally observed properties[26]. The use of conventional LDA and GGA exchange correlation functionals in ceria leads to self interaction error and failure to reproduce the insulating character of defect-free ceria. This necessitates adding a Hubbard potential (U ) correction for the Ce 4f electrons to generate the experimentally observed band gap[27]. Hybrid functionals yield improvement in the electronic picture of ceria, but do not significantly change the energetics of vacancy formation[28]. The effects of transition and rare earth metal dopants[29, 30, 31]: both aliovalent[32, 33] and isovalent[34, 35] on oxygen vacancy formation have been investigated using a supercell approach. The oxygen storage capacity is correlated to the structural relaxation brought about by dopants with smaller ionic radius than Ce4+ and electrostatic effects. Activation energies for potential vacancy migration pathways have been computed from first principles[36, 37, 38] to understand the mechanisms of defect migration at atomistic scale. With the development of density functional perturbation theory, lattice dynamical properties, Born effective charges and phonon density of states have been calculated and these are found to agree well with experimental data[39, 40]. However, ab initio calculations are currently intractable for system sizes greater than a few hundred atoms. To obtain finite temperature bulk properties, it is necessary to move beyond the realm of DFT calculations to statistical thermodynamics of larger system sizes (> 103 atoms). While literature abounds with experimental investigations of the properties of ceria at high temperatures, the computational work described above has been primarily limited to studying the electronic structure and defect formation energies of ceria at absolute zero without attempting to obtain ther-.

(28) 11 modynamic properties at higher temperatures, which is where its most interesting applications and properties emerge.. Our computational study aims to isolate and focus on the thermodynamics of intrinsic oxygen vacancies in ceria relevant to thermochemical cycling. While vacancies are central to the thermochemical cycling process, the thermodynamic driving force is governed by the change in δ (i.e. ∆δ) between TH and TL . For repeatability of the redox cycle, it is necessary to operate in the regime of single phase non-stoichiometric ceria. Furthermore, at such high values of δ, defect interactions become considerable and can negatively impact the entropic driving force for the reduction of ceria. Understanding the nature of vacancy interactions as a function of temperature and concentration in ceria will therefore be instrumental in motivating the exploration of dopants used to improve its suitability. Aside from its immediate relevance to thermochemical fuel production, we chose ceria as our model system since its phase diagram and vacancy thermodynamics are established experimentally. This would help test the accuracy of the computational thermodynamics approach to studying non-stoichiometric oxides, and extend it to screen dopants and predict the properties of doped ceria, for which literature is not as extensive.. Modeling of ceria presents a unique challenge: it requires the ability to capture electron-localization and associated electronic entropy effects. A step in this direction was made for the Lix FePO4 system[41] by showing that including electronic entropy via a cluster expansion approach yields a phase diagram whose topology is in qualitative agreement with experiments. We build upon this effort and seek to conclusively demonstrate the thermodynamic validity of such an approach, by verifying that the inclusion of both electronic and vibrational entropies results in excellent quantitative agreement with experiments for not only the phase diagram, but other thermodynamic quantities as well, such as the entropy of reduction and short-range order..

(29) 12. 2.3. Methodology. The standard first principles approach to computing phase equilibria has been documented for alloys and solid solutions[42, 43, 44]. We present a brief overview here to highlight salient features of this approach relevant to non-stoichiometric oxides. Phase equilibria studies from first principles integrate both rigorous first principles calculations over selected small structures and large scale statistical ensemble based methods. The partition function, which contains all the thermodynamic information for a system, can be coarse grained over a hierarchy of degrees of freedom as described in Equation 2.1. Z=. XX. exp [−βE(σ, ν)] ,. (2.1). σ∈L ν∈σ. where ν,σ are respectively the vibrational and configurational states of the system constrained to a lattice L. Here, the configurational states include both genuine configuration variables (location of oxygen vacancies) and electronic state information (location of Ce3+ ions). The coarse graining takes advantage of the Born Oppenhiemer approximation to separate electronic and nuclear motion in the Hamiltonian. The energy E(σ, ν) is obtained by first computing the electronic ground state for a fixed composition in the lattice, followed by ionic relaxation (once the electrons are thermalized about fixed nuclear positions, they can be assumed to re-equilibrate instantaneously when the nucleii are perturbed). Vibrational frequencies of the system are then calculated for small displacements away from the relaxed ground state at 0 K. The cluster expansion then parametrizes this information in terms of larger structural units and enables estimation of energies of cells and compositions inaccessible through first principles calculations in a fast and efficient manner. Finally, the thermodynamic integration procedure, with the aid of Monte Carlo simulations, incorporates the effect of compositional fluctuations and temperature on the properties of the system and is used to derive other thermodynamic quantities..

(30) 13. 2.3.1. First principles calculations. Electronic structure calculations were performed using the Vienna ab initio simulation package (VASP), a plane wave pseudopotential based DFT code[45]. GGA exchange correlation functional using the PAW (projector augmented wave) method[46] was employed. To correct for the strong on-site coulombic interaction of the Ce 4f electrons, we adopted the rotationally invariant GGA+U formalism introduced by Dudarev et al[47]. The Hubbard potential term ‘U ’ penalizes partial occupancy of the f states and opens up a band gap. The value of U is typically set by fitting to experimentally established band gaps, or quantities such as lattice constant and bulk modulus. For non-stoichiometric ceria, based on previous LDA+U and GGA+U studies[25, 27] of oxygen vacancy formation energies and electron localization on Ce3+ , U =5 for GGA+U and U =6 for LDA+U have been proposed as optimal. Spin polarized GGA+U calculations in this work were all performed using U =5.. Defect. Figure 2.1: 2 × 2 × 2 supercell of stoichiometric ceria. calculations were performed on 2x2x2 supercells (Fig. 2.1) of ceria (96 atoms), using a 2x2x2 k -point grid. To sample structures with different vacancy content and configurations, the desired fraction of oxygen atoms were removed from a 96 atom supercell prior to the simulation. Fig. 2.2 shows a subset of the starting structures.

(31) 14. (a). (b). (c). (d). Figure 2.2: 2×2×2 supercells of ceria with (a) 1 vacancy (δ = 0.0313), (b) 2 vacancies (δ = 0.0625), (c) 3 vacancies (δ = 0.0938) and (d) 5 vacancies (δ = 0.1563).. used for defect calculations. Electronic relaxations were performed until the total energy difference was less than 10−4 eV while ionic relaxations were carried out until residual forces less than 0.02 eV/ were achieved. Formation of vacancies in ceria leads to expansion of the lattice resulting from increased coulombic repulsion between the Ce4+ ions and larger ionic radius of Ce3+ . We account for this by performing multiple constant volume relaxations at distinct volumes for each structure. The energy benefit accrued from the volume relaxation is significant, and if overlooked, could lead to erroneous energies predicted with the cluster expansion later on. In all, 36 different configurations of vacancies were studied with compositions ranging from CeO2 to CeO1.75 ..

(32) 15 First principles lattice dynamics calculations were performed to incorporate vibrational effects on phase stability. We used the ‘small displacement’ finite differences method as implemented in VASP 5.2 to compute the Hessian matrix for the structures. Displacements of 0.015 away from the equilibrium relaxed positions were employed. For higher vacancy concentrations, we included structures with both pseudo-randomly dispersed and clustered arrangements to span the configurational dependence of the vibrational frequencies. The force constants output by VASP were used to obtain the dynamical matrix at other q-points and calculate out the phonon density of states (DOS) using Phonopy[48]. Gaussian smearing and an 8x8x8 q-point mesh were employed for the DOS calculation. The vibrational free energy (FVib ) and entropy (SVib ) were evaluated under the harmonic approximation as FV ib (T ) E∗ = + kB T N N. ∞. hν ln 2 sinh g(ν)dν, 2kB T 0 ∂FV ib /N SV ib (T ) , = N ∂T V Z. (2.2) (2.3). where N is the total number of atoms in the system, ν is the frequency of the phonon mode, g(ν) is the phonon density of states.. 2.3.2. Cluster expansion : configurational degrees of freedom. The cluster expansion (CE) Hamiltonian treats configurational disorder by decomposing the energy of a lattice into a basis of clusters (points, pairs, triplets etc.) of lattice sites. Each cluster is a polynomial in occupation variables and has an associated effective cluster interaction (ECI), ‘J’ in Eq. 2.4. The ECIs are obtained by fitting to the database of ab initio energies: E(σ) = J0 +. X i. Ji σi +. X. Jij σi σj + .... (2.4). i6=j. Vacancies are treated as independent species, so any site in the anion sub-lattice can be occupied by an oxygen ion or vacancy. Additionally, we explicitly treat charge state.

(33) 16 disorder in the cation sub-lattice resulting from Ce4+ /Ce3+ (configurational electronic entropy). In order to describe the energetics of this system with two interacting sub-lattices, we use a multicomponent multilattice CE formalism[49, 50] that works in the product basis of cluster functions defined on each sublattice. Despite the presence of four distinct species (O, Vac, Ce3+ , Ce4+ ), constraints of site and charge balance (2[Ce3+ ] = [Vac]) render the system essentially pseudo-binary. Our cluster expansion fit was obtained using the mmaps code in the alloy theoretic automated toolkit (ATAT)[44, 51]. The knowledge of ECIs provides a computationally inexpensive and efficient means to compute the energy of a large system on the fly during Monte Carlo simulations, circumventing the need for time consuming ab initio calculations. As such, the CE fit to ab initio energies is independent of temperature. By cluster expanding phonon free energies in the basis of clusters fit to configurational energies, the ECIs, and consequently the MC data, can be made to include vibrational effects.. 2.3.3. Lattice Monte Carlo simulations : thermodynamic properties. The fundamental external variables of interest to the thermochemical cycling of ceria are temperature (T) and oxygen partial pressure (pO2 ). Its properties are strongly dependent on the oxygen nonstoichiometry, which is uniquely set for a given (T, pO2 ). Thus, ceria lends itself to be conveniently studied by semi-grand canonical Monte Carlo simulations, treating temperature and chemical potential as external variables. A semi-grand canonical ensemble fixes the total number of lattice sites, letting the concentration of individual species fluctuate in response to an an applied temperature or chemical potential change. Consideration of macroscopic charge-neutrality leaves us with one independent chemical potential µ written as : µ = (µV ac − µO2− ) + 2(µCe3+ − µCe4+ ),. (2.5).

(34) 17 where µV ac , µO2− , µCe3+ and µCe4+ denote the chemical potentials of the individual species which are externally imposed. µ can be described as the free energy cost associated with swapping a pair of Ce4+ and O2− with a pair of Ce3+ and V ac. The Grand Potential Φ(µ, T ) with respect to a reference can be obtained by thermodynamic integration along a fixed T or fixed µ path: Z. µ. hN (T0 , µ)i dµ,. (2.6). (hE(T, µ0 )i − µ hN (T, µ0 )i)dβ.. (2.7). Φ(T0 , µ) = Φ(T0 , µ0 ) − µ0. Φ(T, µ0 ) Φ(T0 , µ0 ) = + kB T kB T0. Z. T. T0. hEi is the thermodynamically averaged energy, hN i is the thermodynamically averaged concentration, µ0 and T0 are the reference chemical potential and temperature, and β = 1/kB T . The low temperature and high temperature expansions used to obtain the reference points for integration are not central to this paper and can be found elsewhere[52]. Our MC runs were performed on 5184 atom cells (larger sizes were attempted and found to not affect the results) using the memc2 code from ATAT[49]. Temperature steps of 40 K were used for the MC runs, with 2000 equilibrium passes and 1000 averaging passes at each (T, pO2 ). Simultaneous spin flips were used to maintain charge balance and were constrained to occur within two unit cell distances of each other. It should be noted that the constraint of charge balance alone is not sufficient to guarantee that the system will never undergo a phase separation into multiple spurious ground states that are locally non-charge balanced although the overall simulation cell is. This can occur when the cluster expansion is only fitted to charge-balanced structures, thus providing little guarantee that the extrapolated energy of non-chargebalanced structures is physically meaningful. We avoided this problem by an iterative procedure. Starting with a cluster expansion fitted to charge-balanced structures only, we monitored the simulation for evidence of phase separation into non-chargebalanced structures. Whenever this was observed, the energy of the structure was calculated from first principles and included in the cluster expansion to reduce extrap-.

(35) 18 olation errors from the fit. Since ab initio calculations imposing periodic boundary conditions necessarily enforce charge-neutrality, we used a neutralizing background charge to estimate the energy of non-charge-balanced structures. This ansatz is justified whenever the resulting calculated energies are sufficiently high, so that these configurations are very rarely sampled in equilibrium.. 2.4 2.4.1. Results and discussion First principles calculations. Using GGA+U calculations, the equilibrium lattice constant for stoichiometric ceria was found to be 5.48. The formation of an oxygen vacancy in a 2x2x2 supercell is accompanied by the localization of two electrons onto the 4f states of two Ce atoms with anti-symmetric spins. True ground state convergence in other vacancy structures was tested by assigning different starting spin configurations to the Ce atoms (up or down spin, and their locations) and looking for the lowest energy structure. The 2p5d and 2p-4f energy gaps were 5.3 eV and 2.5 eV respectively. The formation energy for an oxygen vacancy in a 2x2x2 supercell was calculated to be 3.2 eV, agreeing with previous GGA+U studies[24]. We included up to eight vacancies in a 2x2x2 supercell (corresponding to CeO1.75 ) in different configurations. Such defect concentrations, while high, have been shown to exist in ceria under appropriate (T, pO2 ) and are of interest to us. The lattice expansion associated with vacancy formation was evaluated through multiple constant volume relaxations of each configuration and found to be around 2% for CeO1.75 (eight vacancies in a 2x2x2 supercell). The formation energies f (per mole of gaseous oxygen), Evac , of all the structures relative to the defect-free f supercell are plotted in Fig. 2.3. Evac is defined as. f Evac (δ). =2. ECeO2−δ − ECeO2 δ. + EO2 ,. (2.8). where ECeO2−δ and ECeO2 are the ground state energies of supercells with and without vacancies respectively, and EO2 is the energy of a molecule of gaseous oxygen at stan-.

(36) 19 dard state. The convex hull (solid black line) connects the ground state configurations at each composition. 10. 9. f. Evac (eV). 9.5. 8.5. 8. 7.5 0. 0.05. 0.1 δ. 0.15. 0.2. Figure 2.3: Plot of formation energies of various defect structures as defined in Eq. 2.8. The line connecting the ground states at each composition is the convex hull. Phonon density of states computed under the harmonic approximation are plotted in Fig. 2.4. Vacancies are clearly stabilized by vibrations as evidenced by the softening of modes in CeO1.91 (three vacancies in a 2x2x2 supercell) compared to CeO2 . Further, for a given concentration, clustered vacancies had stiffer phonon modes than vacancies dispersed over the supercell.. 2.4.2. Cluster expansion. The optimal cluster expansion fit to the calculated ab initio energies (CE 1) of the 36 relaxed geometries comprised 13 pair and 1 triplet clusters apart from the null and 2 point clusters. Considering that ceria is an ionic compound, it is important to ascertain if the long range electrostatic interactions are adequately described by a short-range cluster expansion. To ascertain this, we fit another cluster expansion (CE 2) to the ab initio energies after subtracting out the coulombic energy term (computed through an Ewald summation). The latter was then cluster expanded in.

(37) 20 60. CeO1.91 CeO2. no of states/supercell. 50 40 30 20 10 0. 0. 2. 4. 6. 8 10 12 Freq in THz. 14. 16. 18. 20. Figure 2.4: Phonon density of states from first principles calculated under the harmonic approximation. Oxygen vacancies lead to softening of vibrational modes in CeO1.91 (three vacancies in a 2x2x2 supercell) compared to CeO2 . the basis of clusters identified by the fit, and added as an energetic correction to the ECIs. The results are illustrated by Fig. 2.5. The pair and triplet cluster ECIs of CE 2 show identical decay characteristics with cluster diameter as CE 1, indicating that electrostatic interactions are captured well by the cluster expansion. The crossvalidation score[44], which provides a measure of the predictive power of a cluster expansion fit, was close to 0.003 eV for both CE 1 and CE 2. In view of these results, we justify using CE 1 for further work, given its higher computational efficiency. The effect of temperature on ECIs was incorporated by cluster expanding the vibrational free energies in the basis of clusters of CE 1. This introduced a temperature dependent correction to 7 clusters (determined via cross-validation) out of a total of 17.. 2.4.3. Monte Carlo simulations. The Ce-O phase diagram in the composition range of Ce2 O3 - CeO2 has been determined by experiments. The low temperature portion of the phase diagram is complicated by the many vacancy ordered phases of composition Cen O2n−m , and is.

(38) 21 ECI vs cluster diameter 0.2. fit to ab-initio energies less electrostatics CE 1 fit to as calculated ab-initio energies. CE 2. ECI(eV) energy(eV). 0.15. 0.1. 0.05. 0. -0.05. pair. 5. 10 diameter(Angstroms) Cluster diameter(Å). triplet. 5. Figure 2.5: ECI vs cluster diameter for a cluster expansion fit to the as-scalculated first principles energies (squares, CE 1). Subtracting the electrostatic energy prior to fitting and later adding it back (as an energetic correction) does not change the variation of ECIs with cluster diameter (filled triangles, CE 2). This indicates that the electrostatic interactions are captured by the cluster expansion and do not need an explicit treatment. not of primary concern to this work. Of interest to us is the high temperature phase diagram and the ability of first principles calculations to predict the miscibility gap and vacancy thermodynamics in single phase non-stoichiometric ceria. A temperature-composition plot along a constant µ trajectory starting from 0 K is shown in Fig. 2.6. Defect free CeO2 , the starting ground state (GS), is stable up to 1300◦ C before oxygen vacancies start to form. With the inclusion of vibrational effects, the onset of vacancies happens at a much lower temperature of 900◦ C, all other variables being the same. Most ab initio phase diagram studies have in the past neglected the non-configurational contributions to defect formation entropy, and these can substantially affect phase stability. In order to accurately predict the miscibility gap, it is necessary to perform simulations from two different starting points for each µ – a heating simulation from the low temperature ordered ground state, and a cooling simulation from the high tem-.

(39) 22 perature disordered phase. At a given temperature, the discontinuity in concentration when the grand potentials from the two runs are equated leads to the miscibility gap. The phase diagram in the composition range of CeO1.8 to CeO2 obtained using this approach is shown in Fig. 2.7. A miscibility gap shows up even in the absence of vibrations, but the temperature scale is off by nearly a factor of two compared to experiments. The solubility limit of vacancies in ceria is underestimated and the miscibility gap is shown to persist up to temperatures as high as 1500◦ C. The temperature dependent cluster expansion provides a closer agreement : the miscibility gap closes at 800◦ C (690◦ C in experiments) and single phase ceria is shown to be stable at higher oxygen nonstoichiometry at any given temperature. The cluster expansion technique was principally intended to model configurational disorder in alloys in which interatomic interactions tend to be much simpler than in insulators or semiconductors. Studies have however expanded its domain of applications to describe the energetics of Li intercalation in battery materials and model charge state disorder through a localized electronic entropy term[41], equilibrium composition profile across interfaces of doped ceria superlattices[53]. This is the first study of the high temperature phase diagram of ceria from first principles. That it captures the thermodynamics and detects a miscibility gap in a correlated electron system is in itself a significant result; the quantitative agreement with experiment upon including the effect of vibrations and electronic entropy shows even more promise. The phase diagram helps identify thermodynamically stable phases at equilibrium, but even in the region of single phase non-stoichiometric ceria, significant short range order can persist leading to deviation of bulk thermodynamic properties from that of an ideal solution. Indeed, this is the case and ceria deviates from an ideal solution model for δ values as low as 0.007. It is characterized experimentally by studying the dependence of nonstoichiometry (or a dependent property thereof, such as electrical conductivity) on the partial pressure of oxygen. It can also be studied by extracting the nonstoichiometry dependence of entropy change associated with vacancy formation. Momentarily disregarding the entropy of gaseous oxygen released upon vacancy formation, the entropy change for the solid phase can be directly eval-.

(40) 23 2200. With vibrations Without vibrations. 2000 1800. T (C). 1600 1400 1200 1000 800 600 400 1.94. 1.96. 1.98. 2. 2-δ. Figure 2.6: A constant µ trajectory MC simulation starting from the low temperature ground state (CeO2 ) illustrating vibrational effects on the phase diagram and vacancy concentrations. uated by converting the grand canonical output of MC simulations into canonical quantities: hSi =. X 1 (hEi − Φ − µi hni i). T i. (2.9). We fit a model which includes ideal configurational entropy with a polynomial correction term (to account for non-ideal behavior) to S(δ) evaluated per site. δ δ δ δ SSolid (δ) = A 2 ln +2 1− ln 1 − 2 2 2 2 + (2δ) ln (2δ) + (1 − 2δ) ln (1 − 2δ). (2.10). +Bδ 3 + Cδ 2 + Dδ + E, where δ is the non-stoichiometry and A,B,C,D and E are constants (for a given T). The solid state entropy SSolid (δ) per site referenced to SSolid (δ = 0) is plotted in Fig. 2.8 for T=1480 K. The ideal solution entropy (the term whose coefficient is A) peaks at δ = 0.25, but the actual entropy of the system plateaus much sooner. The pronounced deviation from ideal solution behavior is apparent from δ values as low.

(41) 24 1800. MC without vibrations MC with vibrations Experimental. 1600 1400. T(°C). 1200 1000 800 600 400 200. 1.8. 1.85. 1.9 2−!. 1.95. 2. Figure 2.7: (Color online) Miscibility gap in ceria calculated from Monte Carlo simulations. The pronounced effect of vibrations is visible from the suppression of the miscibility gap to lower temperatures and enhanced vacancy solubility in nonstoichiometric ceria. The experimental phase diagram[18] has been overlaid for comparison. as 0.01. Vibrations clearly increase the entropic advantage to having vacancies, but the strongly non ideal character persists. To compare with experimental work[1], we computed the entropy of reduction associated with forming an oxygen vacancy in the limit of infinitesimal change in nonstoichiometry. 1 1 1 CeO2−δ −→ CeO2−(δ+∆δ) + O2 ∆δ→0 ∆δ ∆δ 2. (2.11). ∆ST otal (δ) = ∆SSolid (δ) + 0.5 ∗ SO2 (δ) h p i O2 SO2 (T ) = SO0 2 (T, 1 atm) − kB ln 1 atm 1 ∆SSolid (δ) = (SCeO2−δ − SCeO2−δ−∆δ ) ∆δ. (2.12). lim. (2.13) (2.14). The solid state entropy is readily available from MC simulations. However, there are.

(42) 25 difficulties associated with calculating entropy of gaseous oxygen from first principles, mainly concerned with the definition of a reference state. This can be resolved by using the standard state entropy data for molecular oxygen from thermochemical tables[54]. pO2 can be obtained using Eq. 2.15: µO (T ) = µ0O (T ) + kB T ln. h p i O2 1 atm. (2.15). While the chemical potentials of the respective species from MC simulations are guaranteed to yield the right equilibrium composition and free energies, they are arbitrarily displaced from their true values by an additive constant. This prevents a straightforward application of Equation 2.15. As a workaround, we used the experimentally published nonstoichiometry vs ln(pO2 ) data[1] to fit the chemical potential from MC and obtain the offset. ∆ST otal (δ) computed using this approach at 1480 K is illustrated in Fig. 2.9. The strong deviation from ideal solution model suggests that. 1. S(kB/site). 0.8. MC with vibrations MC without vibrations Ideal solution. 0.6 0.4 0.2 0 0. 0.05. 0.1. 0.15. 0.2. ! Figure 2.8: Entropy of CeO2−δ referenced to CeO2 computed from MC simulations at 1480 K. The deviation from ideal solution behavior (configurational disorder in Ce3+ /Ce4+ and O2− /Vac lattice) becomes apparent even at low δ. Vibrations provide entropic benefit to forming vacancies, but the marked non-ideal behavior prevails. the entropic benefit from vacancies is being offset by some kind of defect interactions..

(43) 26. 70. MC with vibrations MC without vibrations Experiment. "S(kB/atom). 60 50 40 30 20 10 0. 0.05. 0.1. 0.15. 0.2. ! Figure 2.9: Entropy change associated with forming an oxygen vacancy (see Eqn. 2.11) as a function of nonstoichiometry compared with experiment[1]. These defect interactions could arise from stable defect complexes or vacancy ordering over short length scales. We look to characterize and quantify the short range order (SRO) by calculating the thermally averaged pair correlations for the pair clusters in real space. Formally, this idea is embodied in the Warren-Cowley parameters: hσ000 σlmn i − hσ000 i2 αlmn (δ) = , 1 − hσ000 i2 hσ000 σlmn i =. X σ. P (σ, T ). (2.16). 1 X σi σi+(lmn) . N i. (2.17). For a pair {(0,0,0), (l,m,n)} in the O2− /Vac sub-lattice with vacancy site fraction ‘s’, σ ˆi is the occupation variable for site i averaged over all sites equivalent by symmetry, hˆ σ000 i2 = (1 − 2s)2 is the MC average of the point cluster correlation and hˆ σ000 σ ˆlmn i is the averaged correlation function of the pair cluster. P(σ,T) is the probability of configuration σ, given by " 1 P (σ, T ) = exp −β Z({µi }, T ). !# E(σ) −. X i. µ i xi. ,. (2.18).

(44) 27 where Z({µi }, T ) is the semi-grand canonical partition function and {µi } is the set of chemical potentials. If vacancies behave ideally (non interacting, randomly distributed), then hˆ σ000 σ ˆlmn i = hˆ σ000 i hˆ σlmn i = (1 − 2s)2 and αlmn (δ) = 0 for any δ. Clustering of like species is given by αlmn > 0 and likewise ordering of unlike species is given by αlmn < 0.. Figure 2.10: Different vacancy pairs in the anion sub-lattice of a unit cell of ceria. Black boxes denote vacancies. The color scheme for the oxygen atoms corresponds with that used for plotting SRO parameters of various vacancy pairs in Fig. 2.11. Fig. 2.10 shows three vacancy pairs in the anion sublattice of a unit cell of ceria. There are 2 distinct 1/2[111] clusters, one within the unit cell and another extending out of the unit cell, with a face centered Ce atom halfway in between. Tab. 2.1 summarizes the coordinates and diameters of the five smallest pair clusters in the anion sublattice. In Fig. 2.11a, α(δ) at 1320 K for the five clusters in Table 2.1 are plotted. Close to stoichiometry, αlmn = 0 for all (lmn), as would be expected for non interacting vacancies. However, deviations from zero become apparent even for slightly off-stoichiometric compositions. In particular, there is strong preference for vacancies to align along 1/2[110]. The negative correlation along 1/2[100] indicates that two vacancies are not thermodynamically favored at nearest neighbor sites. The.

(45) 28 Table 2.1: Cluster type, coordinates and diameter of the first five pair clusters in the anion sublattice of ceria. There are two distinct 1/2[111] clusters, one within the unit cell (superscript ‘a’) and another extending out of the unit cell, with a face centered Ce atom halfway in between (superscript ‘b’). Cluster type Sites (fractional Diameter(Å) coordinates) 1/2[100] (0.25,0.25,0.25) 2.74 (0.25,0.25,0.75) 1/2[110] (0.25,0.25,0.25) 3.87 (-0.25,0.25,0.75) 1/2[111]a (0.75,0.75,0.75) 4.75 (0.25,0.25,1.25) b 1/2[111] (0.75,0.75,0.75) 4.75 (0.25,0.25,0.25) [100] (0.75,0.75,0.75) 5.48 (-0.25,0.75,0.75). two distinct 1/2[111] pairs have nearly the same value of α > 0 and hence are possible directions for short range clustering of vacancies. The effect of temperature is to favor disorder (Fig. 2.11b for WC parameters at 1791 K), as can be seen from the fact that αlmn ≈ 0 up to larger nonstoichiometry. At still higher concentrations of vacancies, the αlmn start to deviate from zero and show similar clustering/ordering tendencies along the respective directions. There are multiple related material properties associated with vacancy formation in ceria, hence no one rule can govern the choice of dopants. While ease of vacancy formation is crucial, it is the change in nonstoichiometry between the high and low temperature steps (Eqn. 1.1) that ultimately establishes the oxygen uptake and consequently the amount of hydrogen produced. An important implication of this study is that point defect interactions markedly diminish the entropic driving force for thermochemical cycling of ceria. Doping strategies that help screen vacancies from ‘seeing’ each other would inhibit short range ordering/clustering, but it is important to recognize that this introduces redox inactive species in the system, which might affect the thermodynamic efficiency. The power of the electronic structure calculations lies in the ability to explore interactions at an atomistic level, which, when integrated with.

Show more